Last week in Metal Casting, Part 2 we saw how a sand mould for an aftermarket inlet manifold was formed. Now it’s time to watch the pouring of the aluminium and then see the results. As with the previous parts in this series, the work was being done at the Matilda Foundry in Maryborough, Queensland. The casting is a Funnelweb 2V 351 Ford V8 inlet manifold by Parker Racing.
The aluminium is melted down from ingots. The aluminium most often used by this foundry for sand casting is AA601 (US standard 351). This material can be heat treated and machines well.
The ingots are melted in either a gas furnace (pictured) or an electric furnace. A layer of oxide floats on top; it insulates and keeps the air from the molten alloy.
The temperature of the molten alloy is directly measured with a thermocouple. It needs to be at about 710 degrees C.
What look like oversize soup ladles are used to transfer the molten alloy from the furnace to the mould. With a casting of this size, two pourers are used; they time their pour with a countdown so that both mould runners are filled simultaneously.
Ceramic filters have previously been placed in the runners, preventing any impurities from passing into the casting. The filters also reduce the inclusions of air causing the formation of aluminium oxides.
The mould is filled to the top of the risers and runners, the molten material actually forming an inverted meniscus at the surface. A special powder called Feedex is then placed over the exposed aluminium; this keeps it from the air and also...
...as it burns, keeps the riser material from freezing before the casting has solidified. (This allows the riser to feed material to the shrinking casting.)
The casting is left to cool and then fork-lifted to an area where the sand mould can be broken off. The sand has become very hard and is removed with a hammer...
..and pneumatic chisel. Note the sand falling out of the space between the intake manifold runners.
The bare casting is given a quick onceover with a sandblaster, primarily to remove the casting sand that would otherwise damage the...
...bandsaw that is used to cut off the risers and runners. This material is remelted in the furnace.
A die grinder is then used to remove the casting flash – the thin edges of metal that show the parting line of the sand mould.
The foundry’s work with the casting is then finished – the casting is ready to go to the machine shop to be faced and have holes drilled.
As has been seen from this series, developing the pattern for (say) a new intake manifold isn’t the sort of thing that you whip up overnight, get the sand mould made the next day and then have the finished casting back at your house a day later!
However, knowing exactly how castings are produced in small quantities opens up a range of possibilities that may never before have occurred.